DOI: 10.17188/1475830
title: Materials Data on La5Sm3Ni7AgO20 by Materials Project

description: Sm3La5Ni7AgO20 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are twelve inequivalent Sm3+ sites. In the first Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Sm–O bond distances ranging from 2.29–2.46 Å. In the second Sm3+ site, Sm3+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Sm–O bond distances ranging from 2.30–2.72 Å. In the third Sm3+ site, Sm3+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Sm–O bond distances ranging from 2.29–2.96 Å. In the fourth Sm3+ site, Sm3+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Sm–O bond distances ranging from 2.29–2.91 Å. In the fifth Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Sm–O bond distances ranging from 2.26–2.48 Å. In the sixth Sm3+ site, Sm3+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Sm–O bond distances ranging from 2.30–2.87 Å. In the seventh Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Sm–O bond distances ranging from 2.26–2.55 Å. In the eighth Sm3+ site, Sm3+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Sm–O bond distances ranging from 2.28–2.81 Å. In the ninth Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to six O2- atoms. There are a spread of Sm–O bond distances ranging from 2.28–2.84 Å. In the tenth Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to six O2- atoms. There are a spread of Sm–O bond distances ranging from 2.32–2.70 Å. In the eleventh Sm3+ site, Sm3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sm–O bond distances ranging from 2.33–2.92 Å. In the twelfth Sm3+ site, Sm3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of Sm–O bond distances ranging from 2.30–2.46 Å. There are twenty inequivalent La3+ sites. In the first La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.39–3.00 Å. In the second La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.37–2.90 Å. In the third La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.39–2.98 Å. In the fourth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.35–2.98 Å. In the fifth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–2.97 Å. In the sixth La3+ site, La3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of La–O bond distances ranging from 2.34–2.54 Å. In the seventh La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.35–2.95 Å. In the eighth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–2.96 Å. In the ninth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.37–2.90 Å. In the tenth La3+ site, La3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of La–O bond distances ranging from 2.33–2.58 Å. In the eleventh La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.39–3.00 Å. In the twelfth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.36–3.08 Å. In the thirteenth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.37–2.90 Å. In the fourteenth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–2.90 Å. In the fifteenth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–3.00 Å. In the sixteenth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–2.97 Å. In the seventeenth La3+ site, La3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of La–O bond distances ranging from 2.37–2.54 Å. In the eighteenth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.38–2.89 Å. In the nineteenth La3+ site, La3+ is bonded in a 5-coordinate geometry to five O2- atoms. There are a spread of La–O bond distances ranging from 2.30–2.65 Å. In the twentieth La3+ site, La3+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of La–O bond distances ranging from 2.39–2.85 Å. There are twenty-eight inequivalent Ni+2.14+ sites. In the first Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 15–17°. There are a spread of Ni–O bond distances ranging from 2.00–2.21 Å. In the second Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 16–18°. There are a spread of Ni–O bond distances ranging from 2.01–2.22 Å. In the third Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 17–19°. There are a spread of Ni–O bond distances ranging from 2.01–2.22 Å. In the fourth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share a cornercorner with one AgO6 octahedra, corners with three NiO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 15–27°. There are a spread of Ni–O bond distances ranging from 1.98–2.24 Å. In the fifth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 15–17°. There are a spread of Ni–O bond distances ranging from 2.01–2.22 Å. In the sixth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share a cornercorner with one NiO6 octahedra, corners with three AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 22–31°. There are a spread of Ni–O bond distances ranging from 1.97–2.25 Å. In the seventh Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 15–17°. There are a spread of Ni–O bond distances ranging from 2.01–2.19 Å. In the eighth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share a cornercorner with one NiO6 octahedra, corners with three AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 15–27°. There are a spread of Ni–O bond distances ranging from 1.96–2.26 Å. In the ninth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 16–17°. There are a spread of Ni–O bond distances ranging from 2.01–2.16 Å. In the tenth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share a cornercorner with one NiO6 octahedra, corners with three AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 20–30°. There are a spread of Ni–O bond distances ranging from 1.97–2.22 Å. In the eleventh Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 16–17°. There are a spread of Ni–O bond distances ranging from 2.01–2.15 Å. In the twelfth Ni+2.14+ site, Ni+2.14+ is bonded to six O2- atoms to form NiO6 octahedra that share corners with four NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 16–19°. There are a spread of Ni–O bond distances ranging from 2.01–2.20 Å. In the thirteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share a cornercorner with one NiO6 octahedra, a cornercorner with one AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–62°. There are a spread of Ni–O bond distances ranging from 1.92–2.06 Å. In the fourteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–42°. There are a spread of Ni–O bond distances ranging from 1.95–2.06 Å. In the fifteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share a cornercorner with one NiO6 octahedra, a cornercorner with one AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–61°. There are a spread of Ni–O bond distances ranging from 1.90–2.09 Å. In the sixteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–42°. There are a spread of Ni–O bond distances ranging from 1.94–2.04 Å. In the seventeenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share a cornercorner with one NiO6 octahedra, a cornercorner with one AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–62°. There are a spread of Ni–O bond distances ranging from 1.91–2.05 Å. In the eighteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedral tilt angles are 40°. There are a spread of Ni–O bond distances ranging from 1.95–2.04 Å. In the nineteenth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–44°. There are a spread of Ni–O bond distances ranging from 1.93–2.02 Å. In the twentieth Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share a cornercorner with one NiO6 octahedra, a cornercorner with one AgO6 octahedra, and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–64°. There are a spread of Ni–O bond distances ranging from 1.93–2.06 Å. In the twenty-first Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octahedra and corners with two NiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 37–48°. There are a spread of Ni–O bond distances ranging from 1.96–2.06 Å. In the twenty-second Ni+2.14+ site, Ni+2.14+ is bonded to four O2- atoms to form NiO4 tetrahedra that share corners with two NiO6 octah